Fabrication of electrospun polyacrylonitrile ion-exchange ... Fabrication of electrospun...
Embed Size (px)
Transcript of Fabrication of electrospun polyacrylonitrile ion-exchange ... Fabrication of electrospun...
1. Introduction A conventional ion exchange resin usually has a gel or granular structure, composed of styrene or acrylic material . However, micropore structures within the resin result in lower molecular adsorp- tion/desorption rates, due to diffusion distance. With an increase in the pace of processing, the vol- ume of adsorbed molecules increased, and an increase in the frequency of its application rapidly decreased the efficiency of its ion exchange capa- bility, to the point where it was suitable only for smaller molecules. In addition, micropores in tradi- tional resins are easily blocked, which reduces the effectiveness of purification and decreases the regeneration response rate. Furthermore, the resin
itself is vulnerable to damage due to pressure [2–3]. To tackle the above problems, the fiber structure of the ion exchange filters has undergone significant development in recent years. Compared to resins of other types of gel or granular structure, fiber struc- tured resins are simple to use, thanks to their large surface area, and possess high adsorption capacity, fast ion exchange and regeneration rate, as well as other unique features [4–6]. It is widely used in dyes, precious metals, protein pharmaceuticals and other high value-added materials during the enrichment and purification; it is also used in wastewater and gas decontamination processes. The potential bene- fits and value to researchers cannot be overlooked [7–11].
Fabrication of electrospun polyacrylonitrile ion-exchange membranes for application in lysozym H. T. Chiu1*, J. M. Lin1, T. H. Cheng2, S. Y. Chou2
1Department of Materials Science and Engineering National Taiwan University of Science and Technology, No.43, Keelung Rd., Section 4, Taipei, Taiwan
2Department of Products, Taiwan Textile Research Institute, No. 6, Chengtian Rd., Tucheng City, Taipei County 23674, Taiwan
Received 18 August 2010; accepted in revised form 7 November 2010
Abstract. Ion exchange (IEX) chromatography is commonly used in separation and purification systems. However, micro- pore blockage within its resin structure can easily lead to a reduction in the effectiveness of purification. To tackle this prob- lem, we adopted the concept of membrane separation by combining electrospinning techniques with rapid alkaline hydrolysis to prepare a weak acid IEX nanofibrous membrane (AEA-COOH), consisting of polyethyleneterephthalate (PET) meltblown fabric as a supporting layer, with upper and lower IEX layers consisting of polyacrylonitrile (PAN) nanofibrous membranes. To determine the characteristics of the AEA-COOH membrane, we used the commercial product Sartobind® C IEX membrane as the standard of comparison. Results showed that the base weight and thickness of AEA- COOH were 33 and 64%, relative to Sartobind® C membrane. The thermo-degradable temperature of AEA-COOH mem- brane (320°C) was far higher than that of Sartobind® C (115°C), indicating high thermal stability. Finally, comparisons between the lysozyme adsorption rates and capacity of various IEX membranes confirmed that AEA-COOH was lighter, thinner, faster, possessing higher protein adsorption efficiency than Sartobind® C membrane.
Keywords: polymer membranes, electrospun, nanofiber, ion-exchange, lysozymes adsorption
eXPRESS Polymer Letters Vol.5, No.4 (2011) 308–317 Available online at www.expresspolymlett.com DOI: 10.3144/expresspolymlett.2011.31
*Corresponding author, e-mail: email@example.com © BME-PT
According to previous studies [12–18], electrospin- ning is the only direct, efficient, and continuous method for producing polymer nanofibers showing the most promise and greatest efficiency. Hundreds of polymer nanofibers of various kinds have been developed using electrospinning. Electrospinning polymer processing systems deliver polymer solu- tions to a spin feeder, to form liquid droplets. With the application of a high voltage charge, the electri- cal charge within the polymer mutually excludes and overcomes the surface tension of the solution. The surface of the droplets spray a charged liquid column, which, under the continuous effect of the electric field, quickly spiral downward to form a lashing extension. The resulting nanofiber is a thou- sand times thinner than fibers manufactured using normal micro-spinning technology. As the process continues, the solvent in the solution rapidly evapo- rates. Finally, non-woven membranes of nanometer fiber diameter are collected in the collector plate beneath. By electrospinning, fibers with a diameter between a few dozen to several hundred nanome- ters could be manufactured. When compared to tra- ditional fibers (diameter of 50 microns) under the same volumetric conditions, these fibers had a smaller diameter pore aperture, more densely inter- connected pores and increased porosity. In addition, the specific surface area of nanofibers is approxi- mately 100 times that of normal fibers. Thus, nano - fiber membrane filters, when compared to tradi- tional filters, have a higher throughput, lower loss, lower energy consumption, shorter transmission distance, higher adsorption, faster reaction, as well as other advantages [19–21]. Polyacrylonitrile (PAN) possesses high mechanical strength thanks to the strong hydrogen bonding of its molecular structure. It also exhibits strong chem- ical resistance, excellent acid-proof alkalinity, resistance to sunlight, a diminished susceptibility to humidity, and low cost [22–23]. Thus, it has caught the attention of many researchers, in the past 10 years. It is widely used in the preparation of microfiltration (MF), ultrafiltration (UF) and hol- low fiber membranes [24–26]. In addition, PAN molecular chains carry a cyano group, which can be modified. It is hydrolysable and can be adjusted to achieve functionality in a number of applications. If part of the hydrolysis process could be performed with carboxyl functional groups (–COOH) in a solu-
tion, it could quickly adsorb metal ions, lysozymes, and other molecules. Its unique features include high absorption capacity, fast absorption speed, and good dynamic performance. It is an excellent mate- rial for use in the purification of heavy metal waste- water and lysozymes [27–30]. In this study, we first used electrospinning technol- ogy to prepare PAN/PET/PAN nanofiber composite membrane. The nanofiber was stacked into a 3D reticular fiber structure through cross laying. This gave the membrane a high specific surface area, higher porosity (>80%), and micron size membrane pores. With the use of alkaline hydrolysis tech- niques, high-density carboxyl groups appeared on the surface of PAN nanofibers. This prepared the nanofiber membrane for weak acid ion exchange. During the exchange of ions through the nanofiber membrane shortened the distance in molecular dif- fusion, thereby accelerating the rate of ion exchange and improving adsorption capacity. Scanning elec- tron microscopy, porosity analysis, and Toluidine Blue O (TBO) functional groups detector were used to analyze micro-porous PAN/PET/PAN structure, patterns, pore size, distribution, and density of nano - fiber composite membrane and its functional groups. Finally, the nanofiber composite membrane was compared to commercial product Sartobind® C membrane in order to further explore the different ion exchange membranes in the lysozyme adsorp- tion.
2. Experiments 2.1. Materials Polyacrylonitrile (PAN) yarn (Mw = 120 000, con- taining 93% acrylonitrile and 7% vinylacetate) and dimethylacetamide (DMAc) were purchased from Fortune Industries Inc (Tao-Yuan, Taiwan) and I- Chang Chemical Co., Ltd (Taipei, Taiwan), respec- tively. Sodium hydroxide (NaOH) was from J.T. Baker. Lysozyme and Toluidine Blue O (TBO) were from Sigma. The reagents and solvents were of analytical grade and used without further purifi- cation.
2.2. Electrospinning of polyacrylonitrile Electrospinning device was purchased from Jyi Goang Enterprise Co., Ltd. (Taipei, Taiwan). PAN yarn was dissolved in DMAc at a concentration of 15% (w/v). PAN/DMAc solution was loaded into a
Chiu et al. – eXPRESS Polymer Letters Vol.5, No.4 (2011) 308–317
syringe and delivered to the tip of a 21-gauge stain- less steel nozzle with a syringe pump. The nozzle was connected to a power supply and charged to 26.5 kV. The electrospinning mats were collected on nonwoven PET (basis weight 15 g/m2) and wrapped on a grounded steel sheet. The distance between the tip of the nozzle and the substrate was 15.8 cm, the flow rate was 1ml/h, and the collector rotation rate was 24 cm/s. The nozzle was moving along the y-axis (20 cm), and the frequency was 12 times/min.
2.3. Introduction of anionic moieties into PAN nanofiber membranes
Electrospun PAN nanofiber mats were chemically activated by substituting the nitrile groups with anion carboxylic acid groups as an ion exchange material. First, PAN nanofiber mats were alkaline hydrolyzed by immersion in various concentrations (1N, 2N, 3N) of sodium hydroxide stirred (150 rpm) at different temperatures (25–85°C) for 0–40 min. They were washed out with deionized water until no change in pH was apparent. Finally, the carboxy- lated electrospun PAN nanofiber mat was treated with 0.1M HCl, followed by drying in an oven, at 60°C.
2.4. Characterization of fabrics The morphology and diameter of electrospun PAN nanofiber mats before and after the introduction of the ion-exchange groups were observed using a scanning electron microscope (SEM,